In situ recrystallization of lanthanide coordination polymers: from 1D ladder chains to 1D linear chains
Sun, Jing-Wen; Li, Shang-Ju; Yan, Peng-Fei; Yao, Xu; Li, Guang-Ming; CrystEngComm 18 (2016) 3079–; doi:10.1039/C6CE00182C

data_7224649
_publ_section_title
;
 In situ recrystallization of lanthanide coordination polymers: from 1D
 ladder chains to 1D linear chains
;
_journal_issue                   17
_journal_name_full               CrystEngComm
_journal_page_first              3079
_journal_paper_doi               10.1039/C6CE00182C
_journal_volume                  18
_journal_year                    2016
_chemical_absolute_configuration rm
_chemical_formula_moiety         'C38 H36 Lu O20, C6 N'
_chemical_formula_sum            'C44 H36 Lu N O20'
_chemical_formula_weight         1073.71
_chemical_name_systematic
;
 ?
;
_space_group_IT_number           18
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  'P 2 2ab'
_symmetry_space_group_name_H-M   'P 21 21 2'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_audit_update_record
;
2016-01-23 deposited with the CCDC.
2016-03-21 downloaded from the CCDC.
;
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   20.052(7)
_cell_length_b                   16.350(4)
_cell_length_c                   16.623(4)
_cell_measurement_reflns_used    33741
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      27.75
_cell_measurement_theta_min      3.05
_cell_volume                     5450(3)
_computing_cell_refinement       'RAPID-AUTO (Rigaku 1998 <i>RAPID-AUTO</i>)'
_computing_data_collection       'RAPID-AUTO (Rigaku 1998 <i>RAPID-AUTO</i>)'
_computing_data_reduction        'CrystalClear (Rigaku/MSC, 2002)'
_computing_molecular_graphics    'SHELXTL (Sheldrick, 2008)'
_computing_publication_material  SHELXL-97
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.988
_diffrn_measured_fraction_theta_max 0.988
_diffrn_measurement_device_type  'Rigaku RAXIS-RAPID'
_diffrn_measurement_method       '\w scan'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0756
_diffrn_reflns_av_unetI/netI     0.0699
_diffrn_reflns_limit_h_max       23
_diffrn_reflns_limit_h_min       -23
_diffrn_reflns_limit_k_max       19
_diffrn_reflns_limit_k_min       -19
_diffrn_reflns_limit_l_max       19
_diffrn_reflns_limit_l_min       -19
_diffrn_reflns_number            38445
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         25.00
_diffrn_reflns_theta_min         3.22
_exptl_absorpt_coefficient_mu    1.879
_exptl_absorpt_correction_T_max  0.700
_exptl_absorpt_correction_T_min  0.608
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'ABSCOR (Higashi, 1995)'
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    1.309
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             2152
_exptl_crystal_size_max          0.27
_exptl_crystal_size_mid          0.23
_exptl_crystal_size_min          0.19
_platon_squeeze_details          ' ?'
_refine_diff_density_max         1.349
_refine_diff_density_min         -1.157
_refine_diff_density_rms         0.125
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.03(2)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.076
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     599
_refine_ls_number_reflns         9484
_refine_ls_number_restraints     173
_refine_ls_restrained_S_all      1.070
_refine_ls_R_factor_all          0.0780
_refine_ls_R_factor_gt           0.0584
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0893P)^2^+3.0508P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1549
_refine_ls_wR_factor_ref         0.1698
_reflns_number_gt                6950
_reflns_number_total             9615
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c6ce00182c2.cif
_cod_data_source_block           6
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Orthorhombic' changed to
'orthorhombic' according to
/usr/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 4268 2015-11-12 08:31:59Z antanas 

 Adding full bibliography for 7224648--7224657.cif.
;
_cod_database_code               7224649